Alternative Materials for SOFCs,
Opportunities and Limitations
John T. S. Irvine and Paul Connor
Abstract In this chapter, we highlight some critical aspects of materials for use in
solid oxide fuel cells. In relation to oxide ion conducting electrolytes, we address
topics including clustering of defects in zirconias and the resultant limitations on
ionic conductivity. We also discuss the ionic conduction window for various
electrolyte systems. The positive and negative attributes of different anode
materials are considered, highlighting the opportunities for alternative materials to
be utilised in certain parts of the SOFC system. Some suitable system concepts are
presented and a strategy to optimise performance and durability in the same
electrode structures is presented.
Fuel cell systems are highly efﬁcient energy conversion devices, which produce
high quality power in a clean and silent manner. They are highly scalable and so
can be used to from a decentralised power grid, with careful placement enhancing
efﬁciency do to use for CHP. Solid oxide fuel cells (SOFC) also have fuel
ﬂexibility, allowing a number of chemical energy feedstocks.
J. T. S. Irvine (&) Á P. Connor
School of Chemistry, University of St Andrews,
St Andrews, Fife, KY16 9ST, United Kingdom
J. T. S. Irvine and P. Connor (eds.), Solid Oxide Fuels Cells: Facts and Figures,
Green Energy and Technology, DOI: 10.1007/978-1-4471-4456-4_7,
Ó Springer-Verlag London 2013
The focus of fuel cell systems must be the supply of clean energy, which
requires a whole cycle analysis. When this is done, the direct use of the more
transportable, storable and available hydrocarbon fuels is often the most efﬁcient.
The main technological drivers are listed in the Table 1. To compete with existing
energy conversion devices, fuel cell systems must have high performance (both
power density and efﬁciency), durability, low cost and, to ﬁt in most niches, fuel
ﬂexibility. Whilst there are signiﬁcant engineering challenges to achieve all these
points, they all require careful selection of the component materials in the cells.
2 Practical Constraints for SOFC
The SOFC operates at relatively high (400–1,000 °C) temperatures, as these are
required to get sufﬁcient ionic conduction from the ceramic materials. These high
temperatures coupled with the air and fuel input gases produce both highly oxi-
dising and highly reducing atmospheres inside the cells. The materials used to
form the device must, therefore, be able to stand up to the temperatures used and
the oxidising and reducing nature of the gases. They must still perform their role in
the cell be it electrode, electrolyte or interconnect and they must also last for
upwards of 10,000 h of use under these extreme operating conditions.
There are many types of SOFC based on different materials, but they must all
adhere to a similar set of conditions to make a working cell. The most signiﬁcant
conditions are set out in the Table 2 below.
In terms of durability, all materials must be both stable under operating con-
ditions and not react (signiﬁcantly) with the other cell parts they are in contact
with. Their thermal expansion coefﬁcients (TEC) must also match well enough to
ensure heating and cooling cycles do not damage the cell. The electrodes must
conduct electrons, ions and gases (i.e. be porous) and have reasonable kinetics for
the required electrochemical reactions. The electrolyte must be able to conduct
ions, while keeping electrons and gases separated, all the while being stable in
both the fuel and oxidising atmospheres.
Higher operating temperatures will enhance the conductivity of the components
and hence lower the resistances of the cell and will also typically increase the
kinetics of the various reactions, and so will tend to improve the performance of
the system. This is generally true but only as long as the materials in the stack are
stable. The higher operating, and hence exhaust, temperatures can also be used to
improve total efﬁciency of the system by allowing better use of the waste heat.
Table 1 Technology Drivers
Performance Durability Cost Fuel Flexibility
Materials Materials Manufacture Materials
Microstructure and processing Temperature Materials System management
System management System management
164 J. T. S. Irvine and P. Connor
A good example of this is the Rolls Royce Fuel Cell Systems concept  with the
exhaust fed to a gas turbine, which increases the overall electrical efﬁciency.
Another advantage of moving to higher temperatures is that the ease of the
reforming of hydrocarbons is improved, with less tendency for cracking ,
allowing for better fuel ﬂexibility.
However, the complete SOFC stack must not signiﬁcantly degrade over
extended times, at the operating temperature. It is the limit of material stability that
gives the maximum operating temperature of a fuel cell system. An all-ceramic
based cell may be stable to above 900 °C for considerable times, whereas
700–750 °C seems a practical maximum temperature where metals can be
incorporated into the conduction path of the stack (See ‘‘Challenges Imposed by
Thermochemical Expansion of Solid State Electrochemical Materials’’). These
metals are used as interconnects and/or cell supports, and as metals are easier to
manufacture and have typically higher conductivities, similar performance to all
ceramic cells can be achieved at lower cost and operating temperature. However,
as the temperature comes down so does the speed of many of the reactions in the
cell and so the resistance of any ceramic part will increase. To overcome this, all
the electrolyte, in particular, must become thinner , which, while reducing
material costs, does tend to make the processing more expensive and difﬁcult.
The use of lower temperatures will also slow the rate of most chemical deg-
radation processes and so should also increase cell and stack life. The lower
temperature will slow diffusional processes such as grain coarsening and diffusion
across interfaces, which can lead to solid state reactions. However, some impu-
rities may not be removed at these lower temperatures building up on the elec-
trodes leading to degradation. It should also be noted that lower performance at
lower temperatures may necessitate the use of higher electrochemical loads than
would be required for optimal durability.
The choice of operating temperature will naturally come out of the system
design speciﬁcations, including fuel source, as a compromise between cost, per-
formance and fuel source. In some cases, a material or processing step is chosen
for commercial or IP reasons, such as use of metal interconnects, or of thicker YSZ
Table 2 Desirable characteristics for electrolyte, cathode and anode
Cathode Electrolyte Anode
Electronic Conductor Electronic insulator Electronic Conductor
Ionic Conductor Ionic Conductor Ionic Conductor
Porous Gas Tight Porous
Stable in air at High T Stable in air and fuel at High T Stable in fuel at High T
Ideally also stable in air
No reaction with other cell
No reaction with other cell
No reaction with other cell
Matched TEC Matched TEC Matched TEC
Catalyse O2 reduction Catalyse H2 oxidation
Catalyse fuel processing if
Alternative Materials for SOFCs, Opportunities and Limitations 165
electrolytes, which then sets the operating temperature and then applications found
for the system. In both cases, there is a close relation between material properties
and operating temperatures.
The overriding criterion for a fuel cell/stack is the amount of electric energy it can
supply over a practical lifetime. The time frame depends on a lot of factors but
mainly end use and initial cost. For a long-term stationary generation system,
operating time could be tens of thousands of hours, but may only be hundreds of
hours for small portable units. The causes and rates of the various types of deg-
radation are an area of ongoing study.
A reasonable power density expectation for a (planar) fuel cell is about
500 mW cm-2
at 0.7 V, which corresponds to about 0.7 A cm-2
and so a total cell
resistance of about 0.5 ohm cm-2
. Spreading this resistance equally among the
cell components gives a maximum of about 0.15 ohm cm-2
as targets for each of
the cathode, anode and electrolyte [3–5]. with a little leftover for interconnects and
contact resistances. This speciﬁc resistance, however, does give a good upper limit
for any one component in a stack and so this value will be used for the rest of this
4 Electrolyte Material Selection
The electrolyte, along with the interconnect, has to withstand both highly reducing
and highly oxidising atmospheres at the same time in a working fuel cell. As
summarised in Table 2, it must be stable in both of these environments and also
must not react with the electrodes it is in contact with. It must also be mechanically
robust and dense enough to keep the gases separate. It must also be a purely ionic
conductor over the whole range of partial oxygen pressures (pO2) it experiences.
This is a very taxing set of conditions, which only a few materials satisfy.
The choice and form of electrolyte materials will typically set the style and
operating conditions for the rest of the fuel cell system. Thicker, self-supporting
electrolytes are robust and relatively easy to make, but require higher temperatures
to achieve suitable levels of ionic conductance (i.e. low enough resistance). Lower
temperature operation requires thinner electrolytes, and/or higher conductivity
materials, typically supported on another component of the cell. Where not being
limited by other materials in the cell, thinner electrolytes can also be used at higher
temperatures to improve performance.
The trade-off between material conductivity, temperature and cell thickness is
illustrated the plot below. Using the above cut-off resistance of 0.15 X cm-2
the electrolyte, it is possible to calculate a maximum thickness for any given
166 J. T. S. Irvine and P. Connor
conductivity level, or conversely minimum conductivity for given electrolyte
10; 000 lm cmÀ1 Â 0:15 X cmÀ2
A given preparation thickness of electrolyte can be represented by a horizontal
line (the example is 15 lm, r = 0.01 S cm-1
to give cut-off resistance) with any
material with conductivity above that line would be expected to give reasonable
performance. Using the 15 lm line on the plot as an example YSZ needs to
be over 700 °C to achieve better than 0.15 X cm-2
whereas GDC needs only be
above 450 °C. These two regions are shown as heavier lines. Alternatively, if the
electrolyte material and temperature are deﬁned, the conductivity can be worked,
and hence approximate required electrolyte thickness determined. As always,
higher temperatures give better performance, lower resistance (Fig. 1).
For a good electrolyte, the material must be able to be (cheaply) processed to
form a gas tight membrane. Thicker electrolytes, above about 100 lm, can be
strong enough to support both themselves and the electrodes; however electrolytes
thinner than this need to be supported by another (thicker) layer to achieve the
required mechanical strength and still be gas tight.
Other properties of electrolytes can also impose a maximum operating
temperature to ensure continued operation. Proton conducting oxide electrolytes,
for example decrease in hydration on heating, decreasing proton carrier concen-
tration. Simultaneously, competing conduction mechanisms such as hole elec-
tronic and oxide ionic become more signiﬁcant with temperature. This effectively
Fig. 1 Conductivity plots of various electrolytes and interconnects, with corresponding
thicknesses for a resistance of less than 0.15 ohm cm2
. Based on 6 modiﬁed with data from
. Reproduced here with kind permission from Ó Nature Publishing Group 2001
Alternative Materials for SOFCs, Opportunities and Limitations 167
means that pure protonic behaviour is typically observed only up to 700 °C .
Doped cerates, e.g. Gd–CeO2, and some other materials show signiﬁcant levels of
mixed conduction, with electronic conduction becoming relatively more signiﬁ-
cant with increasing temperature . This increasing electronic conduction
eventually reaches a level that causes unacceptable efﬁciency, which gives a
practical upper limit to operating temperature of say 600 °C. Where the system is
operating at low current or on standby for signiﬁcant periods, losses through non-
electrochemical oxidation of fuel are particularly important. Zirconias do not show
such high temperature limitations and are still the most widely used materials.
5 Zirconia Electrolytes: YSZ/SSZ
Yttria-Stabilised Zirconia (YSZ) is the state-of-the-art electrolyte for most solid
oxide fuel cell systems. This is due to its excellent mechanical and ionic con-
duction properties, despite its conductivity limitations below 750 °C. Also the
development time from new material identiﬁcation, cell design and stack building
and the high cost of any unforeseen problems on the way means that tried and
tested YSZ will remain the electrolyte of choice for a long time to come.
Scandia-Stabilised Zirconia (SSZ) shows higher ionic conductivities than YSZ
, but its high cost and lack of availability, coupled with degradation problems
 have limited its widespread use. Political changes have improved the avail-
ability of scandium, and so increased use in recent years. Scandia zirconias also
have much smaller stability ranges for cubic phase formation than their yttria
analogues; see the equilibrium phase diagrams shown in Fig. 2.
The most ionically conductive phase in zirconia is the cubic ﬂuorite phase,
which is not the stable phase at room temperature for pure zirconia. Doping the
zirconia with larger cations and/or introducing oxygen vacancies makes the cubic
ﬂuorite structure more stable. The dopant is typically a divalent or trivalent ele-
). These vacancies tend to increase the effective ionic size,
making the ﬂuorite phase more stable, and also enhance the ionic conductivity by
creating more sites for ion motion. Comparing the Y2O3 and Sc2O3 systems in
Fig. 2 the inﬂuence of ion size can be seen with a much more extensive cubic
region being observed for the Y2O3 systems as Y is much larger than Zr, whereas
Sc is essentially the same size. The stabilisation of the high temperature cubic
phase which gives the materials their name (Scandia-, Yttria- or Calcia-Stabilised
Zirconias) reduces the stresses from phase changes during heating and cooling,
compared to the unstabilised forms.
The conductivity of stabilised zirconias increases to a maximum with
increasing dopant levels see Fig. 3. Increasing the amount of doping induces more
and more oxygen vacancy formation increasing conductivity. At higher vacancy
levels, however, the vacancies start to interact signiﬁcantly, lowering their
mobility, and so reducing conductivity. In the zirconia system, the maximum is
often not achieved within the cubic phase ﬁeld as transformation to lower
168 J. T. S. Irvine and P. Connor
conductivity polymorphs coincides with the conductivity maximum as dopant
content is decreased, see for example that the highest conductivity in Fig. 3 is
observed for a rapidly cooled composition of 7.7 mol % Y2O3 and that on
annealing this transforms to a two-phase sample with much decreased conduc-
tivity. The best conductivities are typically assumed to occur at about 8 mol %
YSZ (8YSZ), see Fig. 3, and about 11 % for SSZ . For pure systems, both
these compositions are strictly not stable in the cubic phase at lower temperatures,
although chemical interaction between electrodes and electrolyte on processing
might assist in stabilising the cubic polymorph to lower temperature.
Increased dopant levels lower the strength, with tetragonal forms tending to be
much stronger and despite a penalty in conductivity , such compositions are
used in some development programmes, especially where strength and small
particle size are beneﬁcial.
Samples, which are cubic throughout the measured temperature range, basically
show two linear conductivity regions in Arrhenius conductivity plots, Fig. 4. In
co-doped systems, a key observation is that the low-temperature activation energy
decreases and the high-temperature activation energy increases as yttrium content
increases and scandium content decreases . This correlates with the strength of
short-range order as indicated by neutron  and electron diffraction studies .
Although scandia substitution increases conductivity and decreases high-temper-
ature activation energy, it also increases the tendency to short-range ordering at
lower temperatures, resulting in a signiﬁcant increase in activation energy for
conduction. This is attributed to the ionic size of the Sc ion, which favours a lower
coordination number than that associated with ideal ﬂuorite phases. It should also
be realised that Zr, which has similar size to Sc, also prefers a lower coordination
number than is ideal for ﬂuorite hence driving the tendency for short-range order in
Fig. 2 Binary phase diagrams for the Y2O3/ZrO2 and Sc2O3/ZrO2 systems [11, 12]. Reproduced
here with kind permission from Ó Academic Press 1970
Alternative Materials for SOFCs, Opportunities and Limitations 169
6 Doped Ceria Oxides
The doped ceria (CeO2) based electrolytes, most typically Gadolinium doped ceria
(GDC), but also Sm doped (SDC), are probably the next most commonly considered
electrolyte. Ceria has the same ﬂuorite structure as doped zirconia, with a similar
conduction mechanism. However, the ceria ﬂuorite phase is stable at all temperatures
and so the dopants are used purely to increase the vacancy concentration, and hence
conductivity. Ceria-based electrolytes exhibit much better ionic conductivity at
lower temperatures than YSZ, able to operate down to about 500 °C.
The main problem with these ceria-based electrolytes is the increasing elec-
tronic (n-type) conduction under reducing conditions, where Ce4+
is reduced to
. While this starts on the anode side of the electrolyte, it can penetrate through
to the cathode side giving an electronic conduction path through the electrolyte .
This internal current leakage reduces the cell efﬁciency by both using up fuel,
without giving external current, but also the voltage of the cell is reduced, so
lowering power output. While the cell is operating, oxide ions are pumped to the
anode side, and so raise the local oxygen activity (pO2) and decrease the extent of
the ceria reduction and hence electronic conduction. This helps to alleviate some
losses; however, if current is stopped or reduced, fuel is oxidised without yielding
is signiﬁcantly larger than Ce4+
(Ionic radius 1.01 Å vs 0.87 Å) ,
there is also a considerable lattice expansion on reduction. This causes strain inside
the electrolyte, which can lead to mechanical stability problems over time. As the
level of reduction changes with cell load, this mechanical stress will vary during
cell operation, limiting cell life. Again, this stress will change across the elec-
trolyte due to variation in oxygen activity.
Fig. 3 The change in
conductivity as a function of
Y2O3 content zirconia of
unannealed and annealed 5-
11 mol % (s, d) and co-
precipitated 8 mol %
YSZ(h, j) at 1000 °C.
The maximum conductivity
moves from 7.7 to 8.5 mol %
after anealing .
Reproduced here with kind
permission from Ó Elsevier
170 J. T. S. Irvine and P. Connor
The practical maximum temperature for a ceria-based electrolyte is at most
600 °C, at which temperature the reduction causes too much electronic conduc-
tivity and the cell efﬁciency drops too far. Protective layers of zirconia are
sometimes applied to prevent such short circuits
7 Anode Selection
Anodes in SOFCs encounter quite a range of different atmospheres, depending
upon source of fuel gas, degree of reforming or partial oxidation and cleanup
processes. The fuel gas will thus comprise of differing ratios of H2, CO, CH4 and
steam with smaller amounts of higher hydrocarbons, sulphur species, as well as
nitrogen and possibly even oxygen if partial oxidation has been utilised. The car-
bon rich fuels can add extra complications as coke formation is likely. Irreversible
reactions can occur with sulphur species and at high steam contents anode oxi-
dation may occur. The cell will preferably be produced in air, and so the anode
should be stable in both air and the highly reducing fuel environment, although a
change in nature between these environments might be tolerable.
An anode has at least two functional parts: the ‘‘active region’’ or electrochemical
functional layer where the fuel is oxidised, and the current collector region which
removes the electrons but still allows the gas access to the inner active region.
Fig. 4 Arrhenius plot of 8 mol % YSZ, showing two different slopes at high and lower
temperature . Reproduced here with kind permission from Ó Springer New York 1996
Alternative Materials for SOFCs, Opportunities and Limitations 171
Depending on the fuel used there might also be a region in the anode gas path for
a fuel reforming catalyst.
The state-of-the-art anode is the Ni/YSZ cermet (CERamic–METal composite).
This mixture of ionically conducting YSZ ceramic, and both electronically con-
ducting and catalytic Ni metal gives the required anode functionality. It is also
easily formed from a nickel oxide–YSZ composite ceramic framework, which can
be ﬁred in air, followed by an in situ reduction to form the desired Ni–YSZ cermet.
This in situ reduction of NiO to Ni metal has the added advantage of increasing the
porosity of the electrode at the same time aiding gas transport. As the Ni acts as
both current collector and fuel oxidation catalyst, the separation of active region
and current collector is sometimes hard to deﬁne.
Nickel metal has a large TEC, much larger than that of the YSZ electrolyte, and so
needs the YSZ (and pores) to reduce the TEC of the electrode to that of the rest of the
cell. There is also, however, a minimum amount of Ni content required in the electrode
to ensure an electronic conduction path (percolation) through all the Ni particles. This
gives a compromise between enough Ni to percolate, but not too much to give a too
high TEC, while still keeping the electrode porous enough for gas transport.
The strengths of the cermet are its good performance with hydrogen as a fuel
coupled with its excellent current collection, and hence low electrode resistance.
This gives high power density for H2 and reformate fuels. It has catalytic ability
not only to oxidise hydrogen, but to also reform methane as well as being a good
steam reforming catalyst .
It does, however, have signiﬁcant weaknesses. A major problem is the fact it is
not redox stable, with the active Ni metal particles easily oxidised back to NiO.
2Ni þ O2 ! 2NiO
This oxidation can occur on fuel starvation, such as on shut down or simply
through lack of fuel, it can also occur under high steam conditions, such as under
high load. This oxidation has two main effects. The NiO takes up signiﬁcantly
more volume than the Ni, causing stress in the electrode, which can lead to
cracking, eventually affecting the structure of the electrode even the whole cell.
The other effect is the highly catalytically active small Ni particles tend to coarsen
on repeated oxidation and reduction, which leads to a lowering of the active area
of the cell, and hence a drop in performance (Table 3).
Although Ni is a good oxidation catalyst, it is also a good catalyst for the
production of carbon ﬁbres
Table 3 Strengths and
weaknesses of Ni–YSZ
Good current collection Not redox stable
Can reform methane Formation of carbon ﬁbres
Steam reforming catalyst Low sulphur tolerance
Triple phase boundary
172 J. T. S. Irvine and P. Connor
CnH2nþ2 ! C
This carbon builds up inside the porous electrode blocking the gas transport into
the electrode, severely compromising performance. If left unchecked, this can
even physically damage the electrode structure, especially as the carbon often
grows underneath Ni particles. This limits the usefulness of Ni cermets for the
readily available higher hydrocarbon fuels, and requires careful control of con-
ditions, e.g. high steam, even for the lower hydrocarbons.
The other reaction of concern for Ni cermets is
Ni þ S ! NiS
Sulphur is a common impurity in many carbon-based fuels, both as naturally
occurring compounds e.g. in biogas or coal gas and the mercaptans added to
natural gas as an odorant .
The Ni–YSZ electrodes suffer from various degradation mechanisms, but they
mainly affect the triple phase boundary (TPB) in the electrode. This is the region
where the electrons, oxide ions and the fuel gases meet and is the site of the fuel
reduction. In the cermet, this region is limited to the interfaces between Ni and
YSZ particles which are connected to current collector and electrolyte, respec-
tively, and are open to pores. This region is poisoned easily as the electrochemical
activity concentrates impurities.
As the TPB is limited to the contact between Ni and YSZ particles, anything
that changes the size of the Ni particles will change the amount of contact. As the
Ni particle size increases with electrode ageing, and especially redox cycling the
TPB decreases lowering the electrode performance. This is always going to be a
problem for mixed ionic/electronic conducting phases.
8 Oxide Anodes
A number of good alternative single-phase perovskite materials exist as possible
anode materials. These are dimensionally stable (and often even redox stable) and
so can easily be used in solid oxide fuel cells. They have good electrode kinetics
(catalytic) properties and are often both ionic as well as electronic conductors.
Their conductivity can be good for oxides, but not as good as metals (e.g. Ni) and
so they are best used as true anodes, i.e. the electrochemical functional layer but
not are generally not good enough to act as current collectors.
Target conductivity for an electrode is around 100 S cm-1
but this value can be
reduced to as low as 1 S cm-1
through careful morphological design, and careful
use and design of current collection. This allows the use of oxide materials as
anodes, removing the metal content and making a more stable cell.
The most common structural type for possible anode materials is the perovskite
structure. This structure is very ﬂexible, allowing most transition metals to be
included in the structure, but also show good stability and electronic conductivity.
Alternative Materials for SOFCs, Opportunities and Limitations 173
Table 4 shows some elements that can be included in perovskite materials,
highlighting those that would be expected to allow a decrease in coordination
number in the perovskite lattice, and hence afford catalytic behaviour, with the
elements stable in the reducing conditions of an SOFC anode indicated on the
bottom line. The use of these species produce a dimensionally stable anode, that
does not change signiﬁcantly between fully oxidised and fully reduced. This
reduces many degradation and lifetime issues.
A good example is La0.75Sr0.25Cr0.5Mn0.5O3 (LSCM) which shows excellent redox
stability, good conductivity and good electrode kinetics. It has been prepared both by
standard high temperature methods  as well as by impregnation into a porous
framework  and shows comparable performance to Ni–YSZ cermet anodes
especially when prepared with high surface area and with appropriate catalysts .
A particularly important property of LSCM is that it has catalytic activity for
direct oxidation of hydrocarbons, which is more signiﬁcant than its reforming
activity [22, 23]. This is shown in Fig. 5 where similar performance is achieved
with direct methane (b) as with hydrogen (a). This means that it is a direct oxi-
dation catalyst with less dependence on the conversion of fuels to hydrogen, e.g.
via water gas shift or reforming, with the stack or cell.
Fuel choice is an important aspect. Hydrogen is often associated with fuel cells due
to its green credentials and simple chemistry; however, hydrogen has several
practical difﬁculties. It is not widely available, as it tends to only be made in large
quantities where it is needed for a chemical process. Also due to its physical
properties, it is hard to transport and store in an energetically efﬁcient manner.
Also, most H2 produced at present is made from reforming natural gas, and so
there is very little green H2 available.
It is generally more efﬁcient to move natural gas about and use it directly and
efﬁciently. For transportable energy sources, liquid fuels are much more practical,
which also requires the use of hydrocarbon fuels. These can be produced from
renewable (e.g. biomass) sources. With increasing demand and limited supplies
hydrocarbons fuels will become even more expensive, emphasising the importance
of enhanced efﬁciency from devices such as SOFCs.
Table 4 Transition metal elements in a perovskite framework, showing ability to reduce oxide
coordination from 6 and stability in fuel atmosphere
Sc Ti V Cr Mn Fe Co Ni Cu Zn
4 4 4 4 CuII
? 4 ? ? 4
MO4Sq ? CuII
Fuel 4 4 4 4 4 ?
174 J. T. S. Irvine and P. Connor
Hydrocarbons utilisation in a fuel cell can follow several parallel pathways (See
Fig. 6), each with many individual steps. The simplest is direct oxidation, but this
requires good oxidation catalyst anodes, and careful control of fuel conditions, but
releases the most energy as it has no endothermic processes. The most common
method of using hydrocarbon fuels is to reform them by heating them with steam
or CO2. This transforms the fuel to H2 and CO which can be used directly in a fuel
cell or via water gas shift from CO to H2. This is also an endothermic reaction and
so needs a heat input, which preferably can be coupled with the heat given out by
the fuel cell oxidations. A similar process is partial oxidation with air, which be
used to simplify overall system structure. Cracking is the thermal decomposition
of methane and short-chain hydrocarbons to yield carbon and is generally unde-
sirable as this leads to structural disruption of the anode; however, a small degree
of cracking to yield tars can be beneﬁcial .
A fuel cell produces waste heat, carbon dioxide and steam, enabling reforma-
tion directly in stack. This has several merits, simplifying both fuel and heat ﬂow
0 0.5 1 1.5 2 2.5
Current Density (A cm
0 0.5 1 1.5 2 2.5
Current Density (A cm
Fig. 5 V-I polarisation
curves for a cell with an
LSCM anode containing
0.5 wt % Pd and 5 wt %
ceria, a measured in
humidiﬁed H2 (3 % H2O) at:
(s) at 973 K, (D) at 1073 K,
and (e) at 1173 K.
b Measured in humidiﬁed
(3 % H2O) CH4 at: (s) at
973 K and (D) at 1073 K.
Filled points give the power
density . Reproduced
here with kind permission
from Ó The Electrochemical
Alternative Materials for SOFCs, Opportunities and Limitations 175
in a ﬁnished system. Allied to this is the concept of gradual internal reforming,
whereby a relatively dry fuel stream becomes increasingly hydrated, allowing
improved reforming as the fuel passes through the stack or across the cell.
When fuels are oxidised at different electrodes, all these pathways may occur;
however, one or two processes will tend to dominate at a given electrode material,
this is illustrated for certain electrodes in Table 5.
10 Fuel Utilisation
It is fairly common when testing fuel cells to get high efﬁciency in laboratory tests
when running at low fuel utilisation; however, when using a fuel cell stack in a real
system, with real, expensive fuels the utilisation needs to be as high as possible,
ideally more than 80 %. This high fuel utilisation produces large amounts of water
(steam) in the stack, coupled with low levels of fuel. The pO2 at the outlet of the
cell/stack can rise high enough to oxidise a nonredox stable electrode (e.g. Ni-
based electrodes). Therefore, all the system then needs to be designed to cope with
this high steam content. One solution is anode gas recycling, where the cell is run
at a safe degree of utilisation, and part of the outlet stream is recycled back to the
fuel input, giving the fuel a second chance to be utilised. This does add water and
CO2 into the fuel input stream, which will reduce voltage and render the fuel
atmosphere more oxidising. This injection of water can have a positive effect on
reforming and aids capture of waste heat in the system.
Another option is to use redox stable anodes to raise the actual fuel utilisation,
without making the system more complex. This is perhaps one of the best reasons
for the use of redox stable anodes as they can tolerate these high steam conditions.
A practical method to optimise performance and fuel utilisation is to use a two-
stage approach with conventional Ni-based electrodes to get high performance,
followed by a stable oxide electrode to maximise the degree of utilisation of the
fuel. For a system with gradual internal reforming, a graduated electrode could be
used with the bulk of the area of the anode being Ni based, to give good reforming
and performance, with a strip of oxide based anode along the exhaust end of the
anode, where there will be a high steam content and all the fuel is reformed. This
last strip can increase the total fuel utilisation to over 90 % and stay stable.
Fig. 6 Alternative pathways
for hydrocarbon utilisation in
SOFC systems .
Reproduced here with kind
permission from Ó Nature
Publishing Group 2004
176 J. T. S. Irvine and P. Connor
The same effect can be achieved using a serial ﬂow set as below where the gas
ﬂows over the Ni-based cells as the fuel is used up and then some oxide based cells
at the end, Fig. 7a. Another useful scenario is to have an oxide anode in the fuel
inlet position, this might utilise a direct oxidation anode at the inlet, to minimise
reforming shock and initiate gradual internal reforming, with a redox tolerant
anode at the exhaust, Fig. 7b.
Another possibility to improve fuel utilisation using a simple planar stack
design is a series–parallel gas ﬂow system that utilises two different stacks, with
the gas ﬂowing through a standard Ni–YSZ based cell stack ﬁrst, with a reason-
able, but safe utilisation, followed by an oxide based cell stack to extract the last of
the unused fuel from the exhaust.
Anode gas recycle can also be used with these systems to further enhance the
fuel utilisation or to supply the steam for any reforming processes.
11 Simultaneous Optimisation of Performance and Durability
The limiting factor for fuel cell performance is often the extent of triple phase
boundary (TPB) available to be the site of cathode or anode reactions. Whilst the
properties of the materials used, whether cermet, composite oxides or a mixed ion
Table 5 Dominating characteristics for a few selected electrode materials for use in hydrocarbon
Key characteristics of selected hydrocarbon oxidation electrodes
Direct Oxidation Catalysts CeO2, LSCM
Reforming Catalysts Ni
Cracking catalysts Ni
Current Collection Cu, Ni, SrTiO3, Nb2Ti2O6
Mixed Electronic/Ionic Conductors
Fig. 7 Schematic of series
gas ﬂow through several fuel
cells: a—to maximise fuel
utilisation, b—to reduce
reforming temperature shock
at the inlet in addition to
Alternative Materials for SOFCs, Opportunities and Limitations 177
conductor, and the ﬁnal microstructure achieved are important, this may be
dominated by the extent of surface area of the electrode. The principal way to
signiﬁcantly increase the TPB length is to decrease the particle size and the use of
nanomaterials is the best way to get the highest surface area.
For most applications, a fuel cell system must also have a long life. In a lifetime
that may be over 40,000 h, degradation in performance must be small, on the order of
a percent every 1,000 h. In an SOFC, the two largest causes of performance loss
(degradation) is the increase in cell resistance due to new phases at critical interfaces,
and the loss of TPB reducing the active area of the cells. The new phases are typically
formed by the slow reaction of component parts of the cells (and metallic inter-
connect corrosion) to form blocking or resistive materials. The loss of TPB can be
due to impurities building upat interface or due to grain growth of the activeparticles,
to reduce their surface energy. Many of the materials used in an SOFC can react at
very high temperatures, but are typically stable at the lower operating temperature of
the cells. An example of this is LSM and YSZ which can react at high temperature to
form a pyrochlore (La2Zr2O7), which is quite resistive compared to YSZ. This forms
at the interface of the electrolyte and LSM, which is the location of the TPB . The
fact that small particles coalesce and grow when heated is well known (Ostwald
ripening). The atoms in small Ni particles are quite mobile and so the particles tend to
coarsen slowly under SOFC operating conditions. The best way to slow both of these
problems is to use larger particles, which will minimise grain growth, and lowers the
reaction area for any side reactions.
So for high performance, one requires small (nano-) particles but to keep
performance for an appreciable time one needs large, stable particles. This sets two
contradictory demands on microstructure.
An elegant solution to this problem is the in situ formation of nanostructured
materials on the electrodes under fuel cell conditions, especially when this is an
equilibrium process. Such behaviour has been observed in YSZ scaffolds impreg-
nated with Mn containing perovskites . When (La,Sr)Mn0.5Cr0.5O3 is prepared
by solution impregnation onto a YSZ skeleton and sintered in air, it forms a think
uniform coating, Fig. 8a, due to a favourable surface interaction between the
Fig. 8 (La,Sr)Mn0.5Cr0.5O3 impregnated onto a YSZ skeleton after ﬁring at 1250 °C in air,
a (left), after subsequent reduction at 800 °C in 5 % H2, b (middle) and after subsequent
reoxidation in air at 800 °C, c (right) . Reproduced here with kind permission from Ó The
Electrochemical Society 2008
178 J. T. S. Irvine and P. Connor
Mn-containing perovskite and the YSZ. On reducing at 800 °C, the coating trans-
forms to a nanoparticulate structure, Fig. 8b, and this reverts towards a smooth
coating on reoxidation at this temperature, Fig. 8c.
This in situ grown nanostructure was associated with the high performance shown
above in Fig. 5. Clearly, nanostructures that are formed under operating tempera-
tures would be intrinsically more stable than those formed ex situ. Thus, this research
provides an important future strategy in matching performance and durability.
In conclusion, it is important to note that many subtle interplays exist that
determine whether new materials have a role to play in fuel cell systems that might
be used commercially. There are several competing factors to consider and it is
generally inappropriate to consider that one material is a simple ‘‘one size’’ ﬁt to
needs. Instead, it is important to optimise microstructure as well as composition
and to consider pertinent application condition, if one is really identify the
opportunities that overcome the limitations of a particular system.
1. F.J. Gardner, M.J. Day, N.P. Brandon, M.N. Pashley, M. Cassidy, SOFC technology
development at Rolls-Royce. J. Power Sources 86, 122–129 (2000)
2. K. Sasaki, K. Watanabe, Y. Teraoka, Direct-alcohol SOFCs: current-voltage characteristics
and fuel gas compositions. J. Electrochem. Soc. 151, A965–A970 (2004)
3. BCH Steele (1994) Proc 1st European solid oxide fuel cell forum (ed U Bossel) 375–397
4. Brian C.H. Steele, Survey of materials selection for ceramic fuel cells II Cathodes and
anodes. Solid State Ionics 86–88, 1223–1234 (1996)
5. Allan J. Jacobson, Materials for solid oxide fuel cells chem. Mater 22, 660–674 (2010)
6. C. H. Brian Steele Angelika H, Materials for fuel-cell technologies. Nature 414:345–352
7. Angela Kruth, John T.S. Irvine, Water incorporation studies on doped barium cerate
perovskites. Solid State Ionics 162–163, 83–91 (2003)
8. Z. Xinge, M. Robertson, C. Decˆes-Petit, W. Qu, O. Kesler, R. Maric, D. Ghosh, Internal
shorting and fuel loss of a low temperature solid oxide fuel cell with SDC electrolyte.
J. Power Sources 164:668–677 (2007)
9. S.P.S. Badwal, F.T. Ciacchi, D. Milosevic, Scandia-zirconia electrolytes for intermediate
temperature oxide fuel cell operation. Solid State Ionics 136–137, 91–99 (2000)
10. T.I. Politova, J.T.S. Irvine, Investigation of scandia-yttria-zirconia system as an electrolyte
material for intermediate temperature fuel cells. Inﬂuence of yttria content in system
(Y2O3)x(Sc2O3)(11-x)(ZrO2)89. Solid State Ionics 168, 153–165 (2004)
11. H.G. Scott, Phase relationships in the zirconia-yttria system. J. Mater. Sci. 10, 1527–1535
12. F.M. Spiridonov, L.N. Popova, R.Y. Popil’skii, On the phase relations and the electrical
conductivity in the system ZrO2-Sc2O3. J. Solid State Chem. 2, 430–438 (1970)
Alternative Materials for SOFCs, Opportunities and Limitations 179
13. R.D. Shannon, Revised effective ionic radii and systematic studies of interatomic distances in
halides and chalcogenides. Acta Cryst. A32, 751–767 (1976)
14. W. Weppner, Tetragonal zirconia polycrystals: a high performance solid oxygen ion
conductor. Solid State Ionics 52, 15–21 (1992)
15. I.R. Gibson, G.P. Dransﬁeld, J.T.S. Irvine, Inﬂuence of Yttria concentration upon electrical
properties and susceptibility to ageing of Yttria-stabilised Zirconia. J. Europ. Ceram. Soc. 18,
16. John T.S. Irvine, Jeremy W.L. Dobson, Tatiana Politova, Susana García-Martíın, Atef
Shenouda, Co-doping of Scandia–Zirconia electrolytes for SOFCs. Faraday Discuss. 134, 41–
17. I.R. Gibson, J.T.S. Irvine, Study of order/disorder transition in Yttria-stabilised Zirconia by
Neutron Diffraction. J. Mater. Chem. 6, 895–898 (1996)
18. S. Garcia-Martin, D.P. Fagg, J.T.S. Irvine, Characterization of diffuse scattering in Yttria-
stabilized zirconia by electron diffraction and high-resolution transmission electron
microscopy. Chem. Mater. 20, 5933–5938 (2008)
19. A. Atkinson, S. Barnett, R.J. Gorte, J.T.S. Irvine, A.J. McEvoy, M. Mogensen, S.C. Singhal,
J. Vohs, Advanced anodes for high-temperature fuel cells. Nat. Mater. 3, 17–27 (2004)
20. S. Tao, J.T.S. Irvine, A Redox-stable, efﬁcient anode for solid-oxide fuel cells. Nat. Mater. 2,
21. G. Kim, G. Corre, J.T.S. Irvine, J.M. Vohs, R.J. Gorte, Engineering composite oxide SOFC
anodes for efﬁcient oxidation of methane. Electrochem. Solid State Lett. 11, B16–B19 (2008)
22. S. Tao, JTS. Irvine, S.M. Plint (2005) Methane oxidation at redox stable fuel cell electrode
La0.75Sr0.25Cr0.5Mn0.5O3-d. J. Phys. Chem. 110:21771–21776
23. Shanwen Tao, John T.S. Irvine, Catalytic properties of the perovskite
La0.75Sr0.25Cr0.5Mn0.5O3-d in relation to its potential as a solid oxide fuel cell anode
material. Chem. Mater. 16, 4116–4121 (2004)
24. Steven McIntosh, Hongpeng He, Shung-Ik Lee, Olga Costa-Nunes, Venkatesan V. Krishnan,
John M. Vohs, Raymond J. Gorte, An examination of carbonaceous deposits in direct-
utilization SOFC anodes. J. Electrochem. Soc. 151, A604–A608 (2004)
25. A. Mitterdorfer, L.J. Gauckler, La2Zr2O7 formation and oxygen reduction kinetics of the
La0.85Sr0.15MnyO3, O2(g)|YSZ system. Solid State Ionics 111, 185–218 (1998)
180 J. T. S. Irvine and P. Connor